##############################################################################
#                                                                            #
# This CIF contains the data for a data article accepted for                 #
# publication in IUCrData. It conforms to the requirements of                #
# Notes for Authors for IUCrData, and has been                               #
# peer reviewed under the auspices of IUCrData.                              #
#                                                                            #
# Full details of the Crystallographic Information File format               #
# are given in the paper "The Crystallographic Information File (CIF):       #
# a New Standard Archive File for Crystallography" by S. R. Hall, F. H.      #
# Allen and I. D. Brown [Acta Cryst. (1991), A47, 655-685].                  #
#                                                                            #
# The current version of the core CIF dictionary is obtainable from          #
# ftp://ftp.iucr.org/pub/cif_core.dic.                                       #
#                                                                            #
# Software is freely available for graphical display of the structure(s)     #
# in this CIF. For information consult the CIF software page                 #
# http://www.iucr.org/resources/cif/software.                                #
#                                                                            #
# This file may be used for bona fide research purposes within the           #
# scientific community so long as proper attribution is given to the data    # 
# article from which it was obtained.                                        #
#                                                                            #
##############################################################################
data_I
_database_code_depnum_ccdc_archive 'CCDC 1993113'
_audit_creation_method     SHELXL-2017/1
_journal_date_recd_electronic     2019-12-24
_journal_date_accepted     2020-03-27
_journal_name_full     'IUCrData'
_journal_year     2020
_journal_volume     5
_journal_issue      4
_journal_page_first     0
_journal_page_last     0
_journal_paper_category     HI
_journal_paper_doi     10.1107/S2414314620004228
_journal_coeditor_code     BH4049
_publ_contact_author_name     'Fan Changzeng'
_publ_contact_author_address
;
State Key Laboratory of Metastable Materials Science and Technology
Yanshan University
Qinhuangdao 066004
People's Republic of China
;
_publ_contact_author_email     chzfan@ysu.edu.cn
_publ_contact_author_fax     ?
_publ_contact_author_phone     '18533575879'
_publ_section_title
;
Crystal structure of the Al₈Cr₅-type intermetallic Al~7.85~Cr~5.16~
;
loop_
    _publ_author_name
    _publ_author_footnote
    _publ_author_address
    "Geng, Xu" .
;
State Key Laboratory of Metastable Materials Science and Technology
Yanshan University
Qinhuangdao 066004
People's Republic of China
;
    "Wen, Bin" .
;
State Key Laboratory of Metastable Materials Science and Technology
Yanshan University
Qinhuangdao 066004
People's Republic of China
;
    "Fan, Changzeng" .
;
State Key Laboratory of Metastable Materials Science and Technology
Yanshan University
Qinhuangdao 066004
People's Republic of China
;
_publ_section_synopsis
;
An aluminium-deficient γ-brass phase, Al~7.85~Cr~5.16~, was synthesized by
high-pressure sintering and its crystal structure determined.
;
_chemical_name_systematic
;
Octaaluminium pentachromium
;
_chemical_name_common     ?
_chemical_formula_moiety     'Al7.85 Cr5.16'
_chemical_formula_sum     'Al7.85 Cr5.16'
_chemical_formula_iupac     'Al7.85 Cr5.16'
_chemical_formula_weight     479.72
_chemical_melting_point     ?
_chemical_absolute_configuration     ?
_space_group_crystal_system     trigonal
_space_group_name_H-M_alt     'R 3 m :R'
_space_group_name_Hall     'P 3* -2'
loop_
    _space_group_symop_operation_xyz
    'x, y, z'
    'z, x, y'
    'y, z, x'
    'y, x, z'
    'x, z, y'
    'z, y, x'
_cell_length_a     7.8777(5)
_cell_length_b     7.8777(5)
_cell_length_c     7.8777(5)
_cell_angle_alpha     109.566(2)
_cell_angle_beta     109.566(2)
_cell_angle_gamma     109.566(2)
_cell_volume     375.01(7)
_cell_formula_units_Z     2
_cell_measurement_reflns_used     2208
_cell_measurement_theta_min     3.16
_cell_measurement_theta_max     26.34
_cell_measurement_temperature     296(2)
_exptl_crystal_description     graininess
_exptl_crystal_colour     'metallic silver'
_exptl_crystal_size_max     0.127
_exptl_crystal_size_mid     0.063
_exptl_crystal_size_min     0.051
_exptl_crystal_density_diffrn     4.248
_exptl_crystal_density_meas     ?
_exptl_crystal_density_method     ?
_exptl_crystal_F_000     451
_exptl_absorpt_coefficient_mu     8.051
_exptl_absorpt_correction_type     multi-scan
_exptl_absorpt_process_details
;
(SADABS; Bruker, 2015)
;
_exptl_absorpt_correction_T_min     0.4955
_exptl_absorpt_correction_T_max     0.5233
_diffrn_ambient_temperature     296(2)
_diffrn_source     ?
_diffrn_radiation_type     MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_measurement_device_type     'Bruker D8 Venture Photon 100 CMOS'
_diffrn_measurement_method     'φ and ω scans'
_diffrn_detector_area_resol_mean     ?
_diffrn_reflns_number     7330
_diffrn_reflns_av_R_equivalents     0.0897
_diffrn_reflns_av_unetI/netI     0.0334
_diffrn_reflns_theta_min     3.165
_diffrn_reflns_theta_max     26.777
_diffrn_reflns_theta_full     25.242
_diffrn_measured_fraction_theta_max     0.987
_diffrn_measured_fraction_theta_full     0.985
_diffrn_reflns_limit_h_min     -9
_diffrn_reflns_limit_h_max     9
_diffrn_reflns_limit_k_min     -9
_diffrn_reflns_limit_k_max     9
_diffrn_reflns_limit_l_min     -9
_diffrn_reflns_limit_l_max     9
_refine_special_details
;
 Refined as a two-component inversion twin
;
_reflns_number_total     576
_reflns_number_gt     547
_reflns_threshold_expression     'I > 2σ(I)'
_refine_ls_structure_factor_coef     Fsqd
_refine_ls_matrix_type     full
_refine_ls_R_factor_all     0.0760
_refine_ls_R_factor_gt     0.0683
_refine_ls_wR_factor_gt     0.1699
_refine_ls_wR_factor_ref     0.1782
_refine_ls_goodness_of_fit_ref     1.156
_refine_ls_restrained_S_all     1.123
_refine_ls_number_reflns     576
_refine_ls_number_parameters     53
_refine_ls_number_restraints     37
_refine_ls_hydrogen_treatment     undef
_refine_ls_weighting_scheme     calc
_refine_ls_weighting_details
             'w=1/[σ²(Fo²)+(0.0652P)²+19.1482P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_hydrogens     .
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary     ?
_refine_ls_shift/su_max     0.000
_refine_ls_shift/su_mean     0.000
_refine_diff_density_max     1.019
_refine_diff_density_min     -1.274
_refine_ls_extinction_method     none
_refine_ls_extinction_coef     .
_refine_ls_abs_structure_details     'Refined as an inversion twin.'
_refine_ls_abs_structure_Flack     0.3(2)
loop_
    _atom_type_symbol
    _atom_type_description
    _atom_type_scat_dispersion_real
    _atom_type_scat_dispersion_imag
    _atom_type_scat_source
    'Al' 'Al' 0.0645 0.0514
                         'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
    'Cr' 'Cr' 0.3209 0.6236
                         'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
_computing_data_collection
;
APEX3 (Bruker, 2015)
;
_computing_cell_refinement
;
APEX3 (Bruker, 2015)
;
_computing_data_reduction
;
APEX3 and SAINT (Bruker, 2015)
;
_computing_structure_solution
;
SHELXT2014/5 (Sheldrick, 2015a)
;
_computing_structure_refinement
;
SHELXL2017/1 (Sheldrick, 2015b)
;
_computing_molecular_graphics
;
DIAMOND (Brandenburg & Putz, 2017)
;
_computing_publication_material
;
publCIF (Westrip, 2010)
;
loop_
    _atom_site_type_symbol
    _atom_site_label
    _atom_site_fract_x
    _atom_site_fract_y
    _atom_site_fract_z
    _atom_site_U_iso_or_equiv
    _atom_site_adp_type
    _atom_site_calc_flag
    _atom_site_occupancy
    _atom_site_disorder_assembly
    _atom_site_disorder_group
    Al Al1 0.2998(14) 0.2998(14) 0.0928(15) 0.0108(19) Uani d 0.772 . 1
    Cr Cr1 0.2998(14) 0.2998(14) 0.0928(15) 0.0108(19) Uani d 0.228 . 2
    Al Al2 1.3096(13) 0.6646(11) 0.6646(11) 0.0117(19) Uani d 0.5 . 3
    Cr Cr2 1.3096(13) 0.6646(11) 0.6646(11) 0.0117(19) Uani d 0.5 . 4
    Al Al3 0.9238(18) 0.6488(14) 0.6488(14) 0.012(2) Uani d 0.958 . 5
    Cr Cr3 0.9238(18) 0.6488(14) 0.6488(14) 0.012(2) Uani d 0.042 . 6
    Cr Cr4 -0.0434(12) -0.0434(12) -0.0434(12) 0.006(2) Uani d 1 . .
    Cr Cr5 0.6391(8) 0.3060(8) 0.3060(8) 0.0028(10) Uani d 1 . .
    Cr Cr6 1.3001(10) 0.9464(8) 0.9464(8) 0.0108(14) Uani d 1 . .
    Cr Cr7 0.5198(13) 0.5198(13) 0.5198(13) 0.008(2) Uani d 1 . .
    Al Al4 0.5500(17) -0.0607(15) 0.2804(16) 0.018(2) Uani d 1 . .
    Al Al5 0.0366(18) 0.0366(18) -0.313(2) 0.015(3) Uani d 1 . .
_geom_special_details     ?
loop_
    _geom_bond_atom_site_label_1
    _geom_bond_atom_site_label_2
    _geom_bond_site_symmetry_2
    _geom_bond_distance
    _geom_bond_publ_flag
    Al1 Cr5 . 2.611(7) ?
    Al1 Cr5 2 2.611(7) ?
    Al1 Cr6 1_444 2.634(7) ?
    Al1 Cr6 2_444 2.634(7) ?
    Al1 Cr4 . 2.644(11) ?
    Al1 Al4 2 2.654(11) ?
    Al1 Al4 5 2.654(11) ?
    Al1 Al5 . 2.659(17) ?
    Al1 Al1 2 2.665(16) ?
    Al1 Al1 3 2.665(16) ?
    Al1 Cr7 . 2.739(11) ?
    Cr1 Cr5 . 2.611(7) ?
    Cr1 Cr5 2 2.611(7) ?
    Cr1 Cr6 1_444 2.634(7) ?
    Cr1 Cr6 2_444 2.634(7) ?
    Cr1 Cr4 . 2.644(11) ?
    Cr1 Al4 2 2.654(11) ?
    Cr1 Al4 5 2.654(11) ?
    Cr1 Al5 . 2.659(17) ?
    Cr1 Cr7 . 2.739(11) ?
    Al2 Cr6 . 2.604(9) ?
    Al2 Cr7 1_655 2.647(9) ?
    Al2 Al4 6_665 2.656(9) ?
    Al2 Al4 2_656 2.656(9) ?
    Al2 Cr5 3_655 2.754(6) ?
    Al2 Cr5 2_655 2.754(6) ?
    Al2 Al5 2_766 2.930(16) ?
    Al2 Al4 4_655 2.996(10) ?
    Al2 Al4 3_655 2.996(10) ?
    Cr2 Cr6 . 2.604(9) ?
    Cr2 Cr7 1_655 2.647(9) ?
    Cr2 Al4 6_665 2.656(9) ?
    Cr2 Al4 2_656 2.656(9) ?
    Cr2 Cr5 3_655 2.754(6) ?
    Cr2 Cr5 2_655 2.754(6) ?
    Cr2 Al5 2_766 2.930(16) ?
    Al3 Cr5 . 2.572(12) ?
    Al3 Cr6 . 2.606(11) ?
    Al3 Cr4 1_666 2.655(12) ?
    Al3 Cr7 . 2.678(13) ?
    Al3 Al5 1_666 2.758(11) ?
    Al3 Al5 3_666 2.758(11) ?
    Al3 Al4 4_655 2.798(12) ?
    Al3 Al4 3_655 2.798(12) ?
    Cr3 Cr5 . 2.572(12) ?
    Cr3 Cr6 . 2.606(11) ?
    Cr3 Cr4 1_666 2.655(12) ?
    Cr3 Cr7 . 2.678(13) ?
    Cr3 Al5 1_666 2.758(11) ?
    Cr3 Al5 3_666 2.758(11) ?
    Cr3 Al4 4_655 2.798(12) ?
    Cr3 Al4 3_655 2.798(12) ?
    Cr4 Al5 . 2.616(10) ?
    Cr4 Al5 3 2.616(10) ?
    Cr4 Al5 2 2.616(10) ?
    Cr4 Cr6 2_444 2.761(7) ?
    Cr4 Cr6 1_444 2.761(7) ?
    Cr5 Cr7 . 2.603(7) ?
    Cr5 Al4 4_655 2.620(10) ?
    Cr5 Al4 3_655 2.620(10) ?
    Cr5 Al4 5 2.652(9) ?
    Cr5 Al4 . 2.652(9) ?
    Cr5 Al5 2_655 2.683(12) ?
    Cr6 Al5 2_766 2.654(12) ?
    Cr6 Al4 5_666 2.739(11) ?
    Cr6 Al4 1_666 2.739(11) ?
    Cr6 Al5 3_666 2.849(8) ?
    Al4 Al5 2_655 2.693(12) ?
    Al4 Al4 3_655 2.726(5) ?
    Al4 Al4 2_545 2.726(5) ?
loop_
    _geom_angle_atom_site_label_1
    _geom_angle_atom_site_label_2
    _geom_angle_atom_site_label_3
    _geom_angle_site_symmetry_1
    _geom_angle_site_symmetry_3
    _geom_angle
    _geom_angle_publ_flag
    Cr5 Al1 Cr5 . 2 110.4(5) ?
    Cr5 Al1 Cr6 . 1_444 63.75(14) ?
    Cr5 Al1 Cr6 2 1_444 167.7(4) ?
    Cr5 Al1 Cr6 . 2_444 167.7(4) ?
    Cr5 Al1 Cr6 2 2_444 63.75(14) ?
    Cr6 Al1 Cr6 1_444 2_444 119.6(5) ?
    Cr5 Al1 Cr4 . . 112.8(3) ?
    Cr5 Al1 Cr4 2 . 112.8(3) ?
    Cr6 Al1 Cr4 1_444 . 63.1(2) ?
    Cr6 Al1 Cr4 2_444 . 63.1(2) ?
    Cr5 Al1 Al4 . 2 125.5(4) ?
    Cr5 Al1 Al4 2 2 60.5(2) ?
    Cr6 Al1 Al4 1_444 2 131.8(4) ?
    Cr6 Al1 Al4 2_444 2 62.4(2) ?
    Cr4 Al1 Al4 . 2 120.0(3) ?
    Cr5 Al1 Al4 . 5 60.5(2) ?
    Cr5 Al1 Al4 2 5 125.5(4) ?
    Cr6 Al1 Al4 1_444 5 62.4(2) ?
    Cr6 Al1 Al4 2_444 5 131.8(4) ?
    Cr4 Al1 Al4 . 5 120.0(3) ?
    Al4 Al1 Al4 2 5 81.7(5) ?
    Cr5 Al1 Al5 . . 124.0(2) ?
    Cr5 Al1 Al5 2 . 124.0(2) ?
    Cr6 Al1 Al5 1_444 . 65.1(3) ?
    Cr6 Al1 Al5 2_444 . 65.1(3) ?
    Cr4 Al1 Al5 . . 59.1(3) ?
    Al4 Al1 Al5 2 . 76.7(3) ?
    Al4 Al1 Al5 5 . 76.7(3) ?
    Cr5 Al1 Al1 . 2 108.1(2) ?
    Cr5 Al1 Al1 2 2 59.3(2) ?
    Cr6 Al1 Al1 1_444 2 111.0(2) ?
    Cr6 Al1 Al1 2_444 2 59.6(2) ?
    Cr4 Al1 Al1 . 2 59.73(18) ?
    Al4 Al1 Al1 2 2 109.0(2) ?
    Al4 Al1 Al1 5 2 168.2(3) ?
    Al5 Al1 Al1 . 2 110.2(3) ?
    Cr5 Al1 Al1 . 3 59.3(2) ?
    Cr5 Al1 Al1 2 3 108.1(2) ?
    Cr6 Al1 Al1 1_444 3 59.6(2) ?
    Cr6 Al1 Al1 2_444 3 111.0(2) ?
    Cr4 Al1 Al1 . 3 59.73(18) ?
    Al4 Al1 Al1 2 3 168.2(3) ?
    Al4 Al1 Al1 5 3 109.0(2) ?
    Al5 Al1 Al1 . 3 110.2(3) ?
    Al1 Al1 Al1 2 3 60.0000(10)
                              ?
    Cr5 Al1 Cr7 . . 58.2(2) ?
    Cr5 Al1 Cr7 2 . 58.2(2) ?
    Cr6 Al1 Cr7 1_444 . 111.2(3) ?
    Cr6 Al1 Cr7 2_444 . 111.2(3) ?
    Cr4 Al1 Cr7 . . 110.2(4) ?
    Al4 Al1 Cr7 2 . 111.1(3) ?
    Al4 Al1 Cr7 5 . 111.1(3) ?
    Al5 Al1 Cr7 . . 169.4(5) ?
    Al1 Al1 Cr7 2 . 60.89(18) ?
    Al1 Al1 Cr7 3 . 60.89(18) ?
    Cr5 Cr1 Cr5 . 2 110.4(5) ?
    Cr5 Cr1 Cr6 . 1_444 63.75(14) ?
    Cr5 Cr1 Cr6 2 1_444 167.7(4) ?
    Cr5 Cr1 Cr6 . 2_444 167.7(4) ?
    Cr5 Cr1 Cr6 2 2_444 63.75(14) ?
    Cr6 Cr1 Cr6 1_444 2_444 119.6(5) ?
    Cr5 Cr1 Cr4 . . 112.8(3) ?
    Cr5 Cr1 Cr4 2 . 112.8(3) ?
    Cr6 Cr1 Cr4 1_444 . 63.1(2) ?
    Cr6 Cr1 Cr4 2_444 . 63.1(2) ?
    Cr5 Cr1 Al4 . 2 125.5(4) ?
    Cr5 Cr1 Al4 2 2 60.5(2) ?
    Cr6 Cr1 Al4 1_444 2 131.8(4) ?
    Cr6 Cr1 Al4 2_444 2 62.4(2) ?
    Cr4 Cr1 Al4 . 2 120.0(3) ?
    Cr5 Cr1 Al4 . 5 60.5(2) ?
    Cr5 Cr1 Al4 2 5 125.5(4) ?
    Cr6 Cr1 Al4 1_444 5 62.4(2) ?
    Cr6 Cr1 Al4 2_444 5 131.8(4) ?
    Cr4 Cr1 Al4 . 5 120.0(3) ?
    Al4 Cr1 Al4 2 5 81.7(5) ?
    Cr5 Cr1 Al5 . . 124.0(2) ?
    Cr5 Cr1 Al5 2 . 124.0(2) ?
    Cr6 Cr1 Al5 1_444 . 65.1(3) ?
    Cr6 Cr1 Al5 2_444 . 65.1(3) ?
    Cr4 Cr1 Al5 . . 59.1(3) ?
    Al4 Cr1 Al5 2 . 76.7(3) ?
    Al4 Cr1 Al5 5 . 76.7(3) ?
    Cr5 Cr1 Cr7 . . 58.2(2) ?
    Cr5 Cr1 Cr7 2 . 58.2(2) ?
    Cr6 Cr1 Cr7 1_444 . 111.2(3) ?
    Cr6 Cr1 Cr7 2_444 . 111.2(3) ?
    Cr4 Cr1 Cr7 . . 110.2(4) ?
    Al4 Cr1 Cr7 2 . 111.1(3) ?
    Al4 Cr1 Cr7 5 . 111.1(3) ?
    Al5 Cr1 Cr7 . . 169.4(5) ?
    Cr6 Al2 Cr7 . 1_655 150.7(4) ?
    Cr6 Al2 Al4 . 6_665 71.0(2) ?
    Cr7 Al2 Al4 1_655 6_665 108.3(2) ?
    Cr6 Al2 Al4 . 2_656 71.0(2) ?
    Cr7 Al2 Al4 1_655 2_656 108.3(2) ?
    Al4 Al2 Al4 6_665 2_656 141.3(4) ?
    Cr6 Al2 Cr5 . 3_655 128.85(18) ?
    Cr7 Al2 Cr5 1_655 3_655 57.6(2) ?
    Al4 Al2 Cr5 6_665 3_655 159.6(4) ?
    Al4 Al2 Cr5 2_656 3_655 57.9(2) ?
    Cr6 Al2 Cr5 . 2_655 128.85(18) ?
    Cr7 Al2 Cr5 1_655 2_655 57.6(2) ?
    Al4 Al2 Cr5 6_665 2_655 57.9(2) ?
    Al4 Al2 Cr5 2_656 2_655 159.6(4) ?
    Cr5 Al2 Cr5 3_655 2_655 102.2(4) ?
    Cr6 Al2 Al5 . 2_766 56.9(3) ?
    Cr7 Al2 Al5 1_655 2_766 93.8(4) ?
    Al4 Al2 Al5 6_665 2_766 82.8(3) ?
    Al4 Al2 Al5 2_656 2_766 82.8(3) ?
    Cr5 Al2 Al5 3_655 2_766 111.2(3) ?
    Cr5 Al2 Al5 2_655 2_766 111.2(3) ?
    Cr6 Al2 Al4 . 4_655 99.9(3) ?
    Cr7 Al2 Al4 1_655 4_655 103.8(3) ?
    Al4 Al2 Al4 6_665 4_655 57.30(18) ?
    Al4 Al2 Al4 2_656 4_655 123.5(4) ?
    Cr5 Al2 Al4 3_655 4_655 108.9(3) ?
    Cr5 Al2 Al4 2_655 4_655 54.7(2) ?
    Al5 Al2 Al4 2_766 4_655 139.6(3) ?
    Cr6 Al2 Al4 . 3_655 99.9(3) ?
    Cr7 Al2 Al4 1_655 3_655 103.8(3) ?
    Al4 Al2 Al4 6_665 3_655 123.5(4) ?
    Al4 Al2 Al4 2_656 3_655 57.30(18) ?
    Cr5 Al2 Al4 3_655 3_655 54.7(2) ?
    Cr5 Al2 Al4 2_655 3_655 108.9(3) ?
    Al5 Al2 Al4 2_766 3_655 139.6(3) ?
    Al4 Al2 Al4 4_655 3_655 70.8(4) ?
    Cr6 Cr2 Cr7 . 1_655 150.7(4) ?
    Cr6 Cr2 Al4 . 6_665 71.0(2) ?
    Cr7 Cr2 Al4 1_655 6_665 108.3(2) ?
    Cr6 Cr2 Al4 . 2_656 71.0(2) ?
    Cr7 Cr2 Al4 1_655 2_656 108.3(2) ?
    Al4 Cr2 Al4 6_665 2_656 141.3(4) ?
    Cr6 Cr2 Cr5 . 3_655 128.85(18) ?
    Cr7 Cr2 Cr5 1_655 3_655 57.6(2) ?
    Al4 Cr2 Cr5 6_665 3_655 159.6(4) ?
    Al4 Cr2 Cr5 2_656 3_655 57.9(2) ?
    Cr6 Cr2 Cr5 . 2_655 128.85(18) ?
    Cr7 Cr2 Cr5 1_655 2_655 57.6(2) ?
    Al4 Cr2 Cr5 6_665 2_655 57.9(2) ?
    Al4 Cr2 Cr5 2_656 2_655 159.6(4) ?
    Cr5 Cr2 Cr5 3_655 2_655 102.2(4) ?
    Cr6 Cr2 Al5 . 2_766 56.9(3) ?
    Cr7 Cr2 Al5 1_655 2_766 93.8(4) ?
    Al4 Cr2 Al5 6_665 2_766 82.8(3) ?
    Al4 Cr2 Al5 2_656 2_766 82.8(3) ?
    Cr5 Cr2 Al5 3_655 2_766 111.2(3) ?
    Cr5 Cr2 Al5 2_655 2_766 111.2(3) ?
    Cr5 Al3 Cr6 . . 157.4(4) ?
    Cr5 Al3 Cr4 . 1_666 139.3(5) ?
    Cr6 Al3 Cr4 . 1_666 63.3(3) ?
    Cr5 Al3 Cr7 . . 59.4(3) ?
    Cr6 Al3 Cr7 . . 143.2(4) ?
    Cr4 Al3 Cr7 1_666 . 79.9(4) ?
    Cr5 Al3 Al5 . 1_666 123.2(3) ?
    Cr6 Al3 Al5 . 1_666 64.1(3) ?
    Cr4 Al3 Al5 1_666 1_666 57.8(3) ?
    Cr7 Al3 Al5 . 1_666 97.1(3) ?
    Cr5 Al3 Al5 . 3_666 123.2(3) ?
    Cr6 Al3 Al5 . 3_666 64.1(3) ?
    Cr4 Al3 Al5 1_666 3_666 57.8(3) ?
    Cr7 Al3 Al5 . 3_666 97.1(3) ?
    Al5 Al3 Al5 1_666 3_666 109.5(6) ?
    Cr5 Al3 Al4 . 4_655 58.2(3) ?
    Cr6 Al3 Al4 . 4_655 105.2(4) ?
    Cr4 Al3 Al4 1_666 4_655 141.1(3) ?
    Cr7 Al3 Al4 . 4_655 103.4(4) ?
    Al5 Al3 Al4 1_666 4_655 83.5(3) ?
    Al5 Al3 Al4 3_666 4_655 154.2(5) ?
    Cr5 Al3 Al4 . 3_655 58.2(3) ?
    Cr6 Al3 Al4 . 3_655 105.2(4) ?
    Cr4 Al3 Al4 1_666 3_655 141.1(3) ?
    Cr7 Al3 Al4 . 3_655 103.4(4) ?
    Al5 Al3 Al4 1_666 3_655 154.2(5) ?
    Al5 Al3 Al4 3_666 3_655 83.5(3) ?
    Al4 Al3 Al4 4_655 3_655 76.6(5) ?
    Cr5 Cr3 Cr6 . . 157.4(4) ?
    Cr5 Cr3 Cr4 . 1_666 139.3(5) ?
    Cr6 Cr3 Cr4 . 1_666 63.3(3) ?
    Cr5 Cr3 Cr7 . . 59.4(3) ?
    Cr6 Cr3 Cr7 . . 143.2(4) ?
    Cr4 Cr3 Cr7 1_666 . 79.9(4) ?
    Cr5 Cr3 Al5 . 1_666 123.2(3) ?
    Cr6 Cr3 Al5 . 1_666 64.1(3) ?
    Cr4 Cr3 Al5 1_666 1_666 57.8(3) ?
    Cr7 Cr3 Al5 . 1_666 97.1(3) ?
    Cr5 Cr3 Al5 . 3_666 123.2(3) ?
    Cr6 Cr3 Al5 . 3_666 64.1(3) ?
    Cr4 Cr3 Al5 1_666 3_666 57.8(3) ?
    Cr7 Cr3 Al5 . 3_666 97.1(3) ?
    Al5 Cr3 Al5 1_666 3_666 109.5(6) ?
    Cr5 Cr3 Al4 . 4_655 58.2(3) ?
    Cr6 Cr3 Al4 . 4_655 105.2(4) ?
    Cr4 Cr3 Al4 1_666 4_655 141.1(3) ?
    Cr7 Cr3 Al4 . 4_655 103.4(4) ?
    Al5 Cr3 Al4 1_666 4_655 83.5(3) ?
    Al5 Cr3 Al4 3_666 4_655 154.2(5) ?
    Cr5 Cr3 Al4 . 3_655 58.2(3) ?
    Cr6 Cr3 Al4 . 3_655 105.2(4) ?
    Cr4 Cr3 Al4 1_666 3_655 141.1(3) ?
    Cr7 Cr3 Al4 . 3_655 103.4(4) ?
    Al5 Cr3 Al4 1_666 3_655 154.2(5) ?
    Al5 Cr3 Al4 3_666 3_655 83.5(3) ?
    Al4 Cr3 Al4 4_655 3_655 76.6(5) ?
    Al5 Cr4 Al5 . 3 118.81(14) ?
    Al5 Cr4 Al5 . 2 118.81(14) ?
    Al5 Cr4 Al5 3 2 118.81(14) ?
    Al5 Cr4 Cr1 . . 60.7(4) ?
    Al5 Cr4 Cr1 3 . 112.2(3) ?
    Al5 Cr4 Cr1 2 . 112.2(3) ?
    Al5 Cr4 Al1 . . 60.7(4) ?
    Al5 Cr4 Al1 3 . 112.2(3) ?
    Al5 Cr4 Al1 2 . 112.2(3) ?
    Al5 Cr4 Al1 . 2 112.2(3) ?
    Al5 Cr4 Al1 3 2 112.2(3) ?
    Al5 Cr4 Al1 2 2 60.7(4) ?
    Cr1 Cr4 Al1 . 2 60.5(4) ?
    Al1 Cr4 Al1 . 2 60.5(4) ?
    Al5 Cr4 Al1 . 3 112.2(3) ?
    Al5 Cr4 Al1 3 3 60.7(4) ?
    Al5 Cr4 Al1 2 3 112.2(3) ?
    Cr1 Cr4 Al1 . 3 60.5(4) ?
    Al1 Cr4 Al1 . 3 60.5(4) ?
    Al1 Cr4 Al1 2 3 60.5(4) ?
    Al5 Cr4 Al3 . 2_444 63.1(2) ?
    Al5 Cr4 Al3 3 2_444 134.0(6) ?
    Al5 Cr4 Al3 2 2_444 63.1(2) ?
    Cr1 Cr4 Al3 . 2_444 107.2(3) ?
    Al1 Cr4 Al3 . 2_444 107.2(3) ?
    Al1 Cr4 Al3 2 2_444 107.2(3) ?
    Al1 Cr4 Al3 3 2_444 165.2(4) ?
    Al5 Cr4 Al3 . 3_444 134.0(6) ?
    Al5 Cr4 Al3 3 3_444 63.1(2) ?
    Al5 Cr4 Al3 2 3_444 63.1(2) ?
    Cr1 Cr4 Al3 . 3_444 165.2(4) ?
    Al1 Cr4 Al3 . 3_444 165.2(4) ?
    Al1 Cr4 Al3 2 3_444 107.2(3) ?
    Al1 Cr4 Al3 3 3_444 107.2(3) ?
    Al3 Cr4 Al3 2_444 3_444 83.6(4) ?
    Al5 Cr4 Al3 . 1_444 63.1(2) ?
    Al5 Cr4 Al3 3 1_444 63.1(2) ?
    Al5 Cr4 Al3 2 1_444 134.0(6) ?
    Cr1 Cr4 Al3 . 1_444 107.2(3) ?
    Al1 Cr4 Al3 . 1_444 107.2(3) ?
    Al1 Cr4 Al3 2 1_444 165.2(4) ?
    Al1 Cr4 Al3 3 1_444 107.2(3) ?
    Al3 Cr4 Al3 2_444 1_444 83.6(4) ?
    Al3 Cr4 Al3 3_444 1_444 83.6(4) ?
    Al5 Cr4 Cr6 . 2_444 63.93(12) ?
    Al5 Cr4 Cr6 3 2_444 168.5(6) ?
    Al5 Cr4 Cr6 2 2_444 63.93(12) ?
    Cr1 Cr4 Cr6 . 2_444 58.27(18) ?
    Al1 Cr4 Cr6 . 2_444 58.27(18) ?
    Al1 Cr4 Cr6 2 2_444 58.27(18) ?
    Al1 Cr4 Cr6 3 2_444 107.8(4) ?
    Al3 Cr4 Cr6 2_444 2_444 57.5(3) ?
    Al3 Cr4 Cr6 3_444 2_444 124.18(16) ?
    Al3 Cr4 Cr6 1_444 2_444 124.18(16) ?
    Al5 Cr4 Cr6 . 1_444 63.93(12) ?
    Al5 Cr4 Cr6 3 1_444 63.93(12) ?
    Al5 Cr4 Cr6 2 1_444 168.5(6) ?
    Cr1 Cr4 Cr6 . 1_444 58.27(18) ?
    Al1 Cr4 Cr6 . 1_444 58.27(18) ?
    Al1 Cr4 Cr6 2 1_444 107.8(4) ?
    Al1 Cr4 Cr6 3 1_444 58.27(18) ?
    Al3 Cr4 Cr6 2_444 1_444 124.18(16) ?
    Al3 Cr4 Cr6 3_444 1_444 124.18(16) ?
    Al3 Cr4 Cr6 1_444 1_444 57.5(3) ?
    Cr6 Cr4 Cr6 2_444 1_444 111.1(2) ?
    Cr3 Cr5 Cr7 . . 62.3(4) ?
    Al3 Cr5 Cr7 . . 62.3(4) ?
    Cr3 Cr5 Al1 . 3 116.2(4) ?
    Al3 Cr5 Al1 . 3 116.2(4) ?
    Cr7 Cr5 Al1 . 3 63.4(3) ?
    Cr7 Cr5 Al1 . . 63.4(3) ?
    Al1 Cr5 Al1 3 . 61.4(4) ?
    Cr7 Cr5 Cr1 . . 63.4(3) ?
    Cr3 Cr5 Al4 . 4_655 65.2(3) ?
    Al3 Cr5 Al4 . 4_655 65.2(3) ?
    Cr7 Cr5 Al4 . 4_655 110.8(3) ?
    Al1 Cr5 Al4 3 4_655 168.9(3) ?
    Al1 Cr5 Al4 . 4_655 107.8(3) ?
    Cr1 Cr5 Al4 . 4_655 107.8(3) ?
    Cr3 Cr5 Al4 . 3_655 65.2(3) ?
    Al3 Cr5 Al4 . 3_655 65.2(3) ?
    Cr7 Cr5 Al4 . 3_655 110.8(3) ?
    Al1 Cr5 Al4 3 3_655 107.8(3) ?
    Al1 Cr5 Al4 . 3_655 168.9(3) ?
    Cr1 Cr5 Al4 . 3_655 168.9(3) ?
    Al4 Cr5 Al4 4_655 3_655 83.0(5) ?
    Cr3 Cr5 Al4 . 5 121.2(3) ?
    Al3 Cr5 Al4 . 5 121.2(3) ?
    Cr7 Cr5 Al4 . 5 115.6(3) ?
    Al1 Cr5 Al4 3 5 110.7(4) ?
    Al1 Cr5 Al4 . 5 60.5(3) ?
    Cr1 Cr5 Al4 . 5 60.5(3) ?
    Al4 Cr5 Al4 4_655 5 62.3(2) ?
    Al4 Cr5 Al4 3_655 5 129.1(2) ?
    Cr3 Cr5 Al4 . . 121.2(3) ?
    Al3 Cr5 Al4 . . 121.2(3) ?
    Cr7 Cr5 Al4 . . 115.6(3) ?
    Al1 Cr5 Al4 3 . 60.5(3) ?
    Al1 Cr5 Al4 . . 110.7(4) ?
    Cr1 Cr5 Al4 . . 110.7(4) ?
    Al4 Cr5 Al4 4_655 . 129.1(2) ?
    Al4 Cr5 Al4 3_655 . 62.3(2) ?
    Al4 Cr5 Al4 5 . 111.7(5) ?
    Cr3 Cr5 Al5 . 2_655 128.3(4) ?
    Al3 Cr5 Al5 . 2_655 128.3(4) ?
    Cr7 Cr5 Al5 . 2_655 169.4(4) ?
    Al1 Cr5 Al5 3 2_655 107.8(3) ?
    Al1 Cr5 Al5 . 2_655 107.8(3) ?
    Cr1 Cr5 Al5 . 2_655 107.8(3) ?
    Al4 Cr5 Al5 4_655 2_655 76.8(3) ?
    Al4 Cr5 Al5 3_655 2_655 76.8(3) ?
    Al4 Cr5 Al5 5 2_655 60.6(3) ?
    Al4 Cr5 Al5 . 2_655 60.6(3) ?
    Cr3 Cr5 Al2 . 2_545 64.3(2) ?
    Al3 Cr5 Al2 . 2_545 64.3(2) ?
    Cr7 Cr5 Al2 . 2_545 59.1(2) ?
    Al1 Cr5 Al2 3 2_545 60.5(3) ?
    Al1 Cr5 Al2 . 2_545 110.8(3) ?
    Cr1 Cr5 Al2 . 2_545 110.8(3) ?
    Al4 Cr5 Al2 4_655 2_545 125.9(4) ?
    Al4 Cr5 Al2 3_655 2_545 59.2(3) ?
    Al4 Cr5 Al2 5 2_545 170.8(4) ?
    Al4 Cr5 Al2 . 2_545 67.3(2) ?
    Al5 Cr5 Al2 2_655 2_545 123.0(2) ?
    Cr2 Cr6 Al1 . 1_666 149.6(2) ?
    Al2 Cr6 Al1 . 1_666 149.6(2) ?
    Cr3 Cr6 Al1 . 1_666 108.9(3) ?
    Al3 Cr6 Al1 . 1_666 108.9(3) ?
    Al1 Cr6 Al1 1_666 3_666 60.8(4) ?
    Cr2 Cr6 Al5 . 2_766 67.7(4) ?
    Al2 Cr6 Al5 . 2_766 67.7(4) ?
    Cr3 Cr6 Al5 . 2_766 136.9(4) ?
    Al3 Cr6 Al5 . 2_766 136.9(4) ?
    Al1 Cr6 Al5 1_666 2_766 108.0(4) ?
    Al1 Cr6 Al5 3_666 2_766 108.0(4) ?
    Al1 Cr6 Al4 1_666 5_666 59.2(3) ?
    Al1 Cr6 Al4 3_666 5_666 107.4(4) ?
    Al5 Cr6 Al4 2_766 5_666 59.9(3) ?
    Cr2 Cr6 Al4 . 1_666 96.4(3) ?
    Al2 Cr6 Al4 . 1_666 96.4(3) ?
    Cr3 Cr6 Al4 . 1_666 126.1(2) ?
    Al3 Cr6 Al4 . 1_666 126.1(2) ?
    Al1 Cr6 Al4 1_666 1_666 107.4(4) ?
    Al1 Cr6 Al4 3_666 1_666 59.2(3) ?
    Al5 Cr6 Al4 2_766 1_666 59.9(3) ?
    Al4 Cr6 Al4 5_666 1_666 106.5(5) ?
    Al1 Cr6 Cr4 1_666 1_666 58.6(2) ?
    Al1 Cr6 Cr4 3_666 1_666 58.6(2) ?
    Al5 Cr6 Cr4 2_766 1_666 163.9(4) ?
    Al4 Cr6 Cr4 5_666 1_666 113.1(3) ?
    Al4 Cr6 Cr4 1_666 1_666 113.1(3) ?
    Cr2 Cr6 Cr5 . 1_666 127.0(4) ?
    Al2 Cr6 Cr5 . 1_666 127.0(4) ?
    Cr3 Cr6 Cr5 . 1_666 163.9(3) ?
    Al3 Cr6 Cr5 . 1_666 163.9(3) ?
    Al1 Cr6 Cr5 1_666 1_666 57.7(2) ?
    Al1 Cr6 Cr5 3_666 1_666 57.7(2) ?
    Al5 Cr6 Cr5 2_766 1_666 59.2(3) ?
    Al4 Cr6 Cr5 5_666 1_666 57.6(2) ?
    Al4 Cr6 Cr5 1_666 1_666 57.6(3) ?
    Cr4 Cr6 Cr5 1_666 1_666 104.7(3) ?
    Cr2 Cr6 Al5 . 3_666 99.6(3) ?
    Al2 Cr6 Al5 . 3_666 99.6(3) ?
    Cr3 Cr6 Al5 . 3_666 60.5(3) ?
    Al3 Cr6 Al5 . 3_666 60.5(3) ?
    Al1 Cr6 Al5 1_666 3_666 105.5(3) ?
    Al1 Cr6 Al5 3_666 3_666 57.8(3) ?
    Al5 Cr6 Al5 2_766 3_666 127.5(2) ?
    Al4 Cr6 Al5 5_666 3_666 164.0(4) ?
    Al4 Cr6 Al5 1_666 3_666 72.2(3) ?
    Cr4 Cr6 Al5 1_666 3_666 55.6(2) ?
    Cr5 Cr6 Al5 1_666 3_666 111.8(3) ?
    Cr5 Cr7 Cr5 . 3 110.9(2) ?
    Cr5 Cr7 Cr5 . 2 110.9(2) ?
    Cr5 Cr7 Cr5 3 2 110.9(2) ?
    Cr5 Cr7 Al2 . 1_455 166.5(5) ?
    Cr5 Cr7 Al2 3 1_455 63.27(8) ?
    Cr5 Cr7 Al2 2 1_455 63.27(8) ?
    Cr5 Cr7 Al2 . 3_554 63.27(8) ?
    Cr5 Cr7 Al2 3 3_554 166.5(5) ?
    Cr5 Cr7 Al2 2 3_554 63.27(8) ?
    Cr5 Cr7 Al2 . 2_545 63.27(8) ?
    Cr5 Cr7 Al2 3 2_545 63.27(8) ?
    Cr5 Cr7 Al2 2 2_545 166.5(5) ?
    Al2 Cr7 Al2 1_455 2_545 119.39(7) ?
    Al2 Cr7 Al2 3_554 2_545 119.39(7) ?
    Cr5 Cr7 Al3 . . 58.3(2) ?
    Cr5 Cr7 Al3 3 . 124.25(17) ?
    Cr5 Cr7 Al3 2 . 124.25(17) ?
    Cr5 Cr7 Cr3 . . 58.3(2) ?
    Cr5 Cr7 Cr3 3 . 124.25(17) ?
    Cr5 Cr7 Cr3 2 . 124.25(17) ?
    Cr5 Cr7 Al3 . 2 124.25(17) ?
    Cr5 Cr7 Al3 3 2 124.25(17) ?
    Cr5 Cr7 Al3 2 2 58.3(2) ?
    Al2 Cr7 Al3 1_455 2 64.46(17) ?
    Al2 Cr7 Al3 3_554 2 64.46(17) ?
    Al2 Cr7 Al3 2_545 2 135.3(5) ?
    Al3 Cr7 Al3 . 2 82.8(4) ?
    Cr3 Cr7 Al3 . 2 82.8(4) ?
    Cr5 Cr7 Al3 . 3 124.25(17) ?
    Cr5 Cr7 Al3 3 3 58.3(2) ?
    Cr5 Cr7 Al3 2 3 124.25(17) ?
    Cr5 Cr7 Al1 . 3 58.5(2) ?
    Cr5 Cr7 Al1 3 3 58.5(2) ?
    Cr5 Cr7 Al1 2 3 106.2(4) ?
    Al2 Cr7 Al1 1_455 3 110.2(3) ?
    Al2 Cr7 Al1 3_554 3 110.2(3) ?
    Al2 Cr7 Al1 2_545 3 60.3(3) ?
    Al3 Cr7 Al1 . 3 108.7(3) ?
    Cr3 Cr7 Al1 . 3 108.7(3) ?
    Al3 Cr7 Al1 2 3 164.4(4) ?
    Al3 Cr7 Al1 3 3 108.7(3) ?
    Cr5 Cr7 Al1 . 2 106.2(4) ?
    Cr5 Cr7 Al1 3 2 58.5(2) ?
    Cr5 Cr7 Al1 2 2 58.5(2) ?
    Al2 Cr7 Al1 1_455 2 60.3(3) ?
    Al2 Cr7 Al1 3_554 2 110.2(3) ?
    Al2 Cr7 Al1 2_545 2 110.2(3) ?
    Al3 Cr7 Al1 . 2 164.4(4) ?
    Cr3 Cr7 Al1 . 2 164.4(4) ?
    Al3 Cr7 Al1 2 2 108.7(3) ?
    Al3 Cr7 Al1 3 2 108.7(3) ?
    Al1 Cr7 Al1 3 2 58.2(4) ?
    Cr5 Al4 Cr5 2_545 . 144.8(4) ?
    Cr5 Al4 Al1 2_545 3 86.3(4) ?
    Cr5 Al4 Al1 . 3 59.0(3) ?
    Cr5 Al4 Al2 2_545 3_544 62.9(2) ?
    Cr5 Al4 Al2 . 3_544 150.4(5) ?
    Al1 Al4 Al2 3 3_544 148.8(4) ?
    Cr5 Al4 Al5 2_545 2_655 145.4(6) ?
    Cr5 Al4 Al5 . 2_655 60.2(3) ?
    Al1 Al4 Al5 3 2_655 106.3(3) ?
    Al2 Al4 Al5 3_544 2_655 102.4(4) ?
    Cr5 Al4 Al4 2_545 3_655 134.5(5) ?
    Cr5 Al4 Al4 . 3_655 58.3(4) ?
    Al1 Al4 Al4 3 3_655 103.5(4) ?
    Al2 Al4 Al4 3_544 3_655 95.5(4) ?
    Al5 Al4 Al4 2_655 3_655 74.9(5) ?
    Cr5 Al4 Al4 2_545 2_545 59.4(3) ?
    Cr5 Al4 Al4 . 2_545 128.9(4) ?
    Al1 Al4 Al4 3 2_545 102.1(5) ?
    Al2 Al4 Al4 3_544 2_545 67.6(4) ?
    Al5 Al4 Al4 2_655 2_545 86.1(5) ?
    Al4 Al4 Al4 3_655 2_545 151.5(6) ?
    Cr5 Al4 Cr6 2_545 1_444 106.6(5) ?
    Cr5 Al4 Cr6 . 1_444 61.8(2) ?
    Al1 Al4 Cr6 3 1_444 58.4(3) ?
    Al2 Al4 Cr6 3_544 1_444 132.5(4) ?
    Al5 Al4 Cr6 2_655 1_444 58.5(3) ?
    Al4 Al4 Cr6 3_655 1_444 116.5(5) ?
    Al4 Al4 Cr6 2_545 1_444 68.0(3) ?
    Cr5 Al4 Al3 2_545 2_545 56.6(3) ?
    Cr5 Al4 Al3 . 2_545 118.0(5) ?
    Al1 Al4 Al3 3 2_545 97.2(4) ?
    Al2 Al4 Al3 3_544 2_545 62.7(3) ?
    Al5 Al4 Al3 2_655 2_545 147.5(5) ?
    Al4 Al4 Al3 3_655 2_545 78.0(4) ?
    Al4 Al4 Al3 2_545 2_545 110.9(4) ?
    Cr6 Al4 Al3 1_444 2_545 153.0(5) ?
    Cr5 Al4 Al2 2_545 2_545 99.8(4) ?
    Cr5 Al4 Al2 . 2_545 58.0(2) ?
    Al1 Al4 Al2 3 2_545 56.9(3) ?
    Al2 Al4 Al2 3_544 2_545 120.5(4) ?
    Al5 Al4 Al2 2_655 2_545 114.1(4) ?
    Al4 Al4 Al2 3_655 2_545 55.1(2) ?
    Al4 Al4 Al2 2_545 2_545 153.3(5) ?
    Cr6 Al4 Al2 1_444 2_545 106.8(3) ?
    Al3 Al4 Al2 2_545 2_545 61.3(4) ?
    Cr4 Al5 Cr6 . 3_443 152.4(6) ?
    Cr4 Al5 Cr1 . . 60.2(4) ?
    Cr6 Al5 Cr1 3_443 . 147.5(5) ?
    Cr4 Al5 Al1 . . 60.2(4) ?
    Cr6 Al5 Al1 3_443 . 147.5(5) ?
    Cr4 Al5 Cr5 . 3_554 145.1(6) ?
    Cr6 Al5 Cr5 3_443 3_554 62.5(3) ?
    Cr1 Al5 Cr5 . 3_554 84.9(5) ?
    Al1 Al5 Cr5 . 3_554 84.9(5) ?
    Cr4 Al5 Al4 . 6_554 125.1(3) ?
    Cr6 Al5 Al4 3_443 6_554 61.6(3) ?
    Al1 Al5 Al4 . 6_554 102.9(4) ?
    Cr5 Al5 Al4 3_554 6_554 59.1(3) ?
    Cr4 Al5 Al4 . 3_554 125.1(3) ?
    Cr6 Al5 Al4 3_443 3_554 61.6(3) ?
    Cr1 Al5 Al4 . 3_554 102.9(4) ?
    Al1 Al5 Al4 . 3_554 102.9(4) ?
    Cr5 Al5 Al4 3_554 3_554 59.1(3) ?
    Al4 Al5 Al4 6_554 3_554 109.2(5) ?
    Cr4 Al5 Al3 . 2_444 59.1(3) ?
    Cr6 Al5 Al3 3_443 2_444 101.0(4) ?
    Cr1 Al5 Al3 . 2_444 103.8(4) ?
    Al1 Al5 Al3 . 2_444 103.8(4) ?
    Cr5 Al5 Al3 3_554 2_444 138.3(3) ?
    Al4 Al5 Al3 6_554 2_444 149.3(6) ?
    Al4 Al5 Al3 3_554 2_444 79.2(3) ?
    Cr4 Al5 Al3 . 1_444 59.1(3) ?
    Cr6 Al5 Al3 3_443 1_444 101.0(4) ?
    Cr1 Al5 Al3 . 1_444 103.8(4) ?
    Al1 Al5 Al3 . 1_444 103.8(4) ?
    Cr5 Al5 Al3 3_554 1_444 138.3(3) ?
    Al4 Al5 Al3 6_554 1_444 79.2(3) ?
    Al4 Al5 Al3 3_554 1_444 149.3(6) ?
    Al3 Al5 Al3 2_444 1_444 79.9(6) ?
    Cr4 Al5 Cr6 . 1_444 60.5(3) ?
    Cr6 Al5 Cr6 3_443 1_444 126.6(2) ?
    Cr1 Al5 Cr6 . 1_444 57.0(2) ?
    Al1 Al5 Cr6 . 1_444 57.0(2) ?
    Cr5 Al5 Cr6 3_554 1_444 101.9(3) ?
    Al4 Al5 Cr6 6_554 1_444 66.8(2) ?
    Al4 Al5 Cr6 3_554 1_444 155.4(6) ?
    Al3 Al5 Cr6 2_444 1_444 117.2(4) ?
    Al3 Al5 Cr6 1_444 1_444 55.4(2) ?
    Cr4 Al5 Cr6 . 2_444 60.5(3) ?
    Cr6 Al5 Cr6 3_443 2_444 126.6(2) ?
    Cr1 Al5 Cr6 . 2_444 57.0(2) ?
    Al1 Al5 Cr6 . 2_444 57.0(2) ?
    Cr5 Al5 Cr6 3_554 2_444 101.9(3) ?
    Al4 Al5 Cr6 6_554 2_444 155.4(6) ?
    Al4 Al5 Cr6 3_554 2_444 66.8(2) ?
    Al3 Al5 Cr6 2_444 2_444 55.4(2) ?
    Al3 Al5 Cr6 1_444 2_444 117.2(4) ?
    Cr6 Al5 Cr6 1_444 2_444 106.1(4) ?
    Cr4 Al5 Al2 . 3_443 97.0(4) ?
    Cr6 Al5 Al2 3_443 3_443 55.3(3) ?
    Cr1 Al5 Al2 . 3_443 157.2(5) ?
    Al1 Al5 Al2 . 3_443 157.2(5) ?
    Cr5 Al5 Al2 3_554 3_443 117.9(4) ?
    Al4 Al5 Al2 6_554 3_443 90.1(4) ?
    Al4 Al5 Al2 3_554 3_443 90.1(4) ?
    Al3 Al5 Al2 2_444 3_443 59.8(3) ?
    Al3 Al5 Al2 1_444 3_443 59.8(3) ?
    Cr6 Al5 Al2 1_444 3_443 113.8(3) ?
    Cr6 Al5 Al2 2_444 3_443 113.8(3) ?
_shelx_space_group_comment     ?
_shelx_estimated_absorpt_T_min     ?
_shelx_estimated_absorpt_T_max     ?
